Identification of changes in the microstructure of damaged elements spherical joint
International Journal of Engineering Inventionse-ISSN: 2278-7461, p-ISSN: 2319-6491Volume 2, Issue 6 (April 2013) PP: 38-43www.ijeijournal.com Page | 38Identification of changes in the microstructure of damagedelements spherical jointMr. Sc. Mujanović Enes1, Dr. Sc. Denijal Sprečić21,2University of Tuzla, Faculty of Mechanical Engineering, Univerzitetska Str. 4, 75000 Tuzla,Bosnia and HerzegovinaAbstract: Spherical joint are a special kind of mechanisms which serve to transmit the torque and the forcebetween the individual aggregates, respectively, in which case their shafts, connected with this gear, are undercertain constant angle or under a variable (changing) angle during the operation. These gear are widely used inautomobile industry. The main characteristic of these gears in that during the torque transmission relativemoving (displacing) in allowed, which can be under an angle or translatory and that, except for purelymechanical losses, there are no other losses such as may be the torque inscrease or decrease. During theoperation damages occur on the parts (elements) of hinged gear. For this reason the analysis of themicrostructure is essntial to establish the causes and to decrease the damages on the observed parts.Keywords: Mechanism, spherical joint, universal joint, microstructure, machine vision.I. INTRODUCTIONThe main parts of the universal joint are shaft and the hinged coupling. The Universal joints can haveone or more hinged couplings. The wide application and diversity of functional requirements conditioned thecreation of a high number of types of hinged couplings (spherical joints) of different constructions (designs), theconstruction of a hinged coupling influencing the construction of universal joint. The hinged couplings arebasically divided into asynchronous and synchronous hinged couplings. The asynchronous hinged couplingsmake possible the periodic variability of the angle velocity of the driven shaft, while the synchronous couplingsensure a constant angle velocity of the outlet (driven) shaft, under the variable (changing) and relatively bigoperating angles between the shafts.II. THE ELEMENTS OF THE TRANSMISSION OF THE UNIVERSAL JOINTThe basic characteristic of the asynchronous gears is the periodic variability of the angle velocity of thedriven shaft, the variability being greater, the greater the angle between the intersecting shafts is.76 54321Figure 1: Universal joint with constituent elementsFrom the group of asynchronous hinged couplings we performed laboratory analyses of the parts of theuniversal joint. The universal joint is constructed in the form of two separate forks firmly connected to bothparts of the shaft. The legs of the forks are turned under the angle of 90oone towards the other and they arehinged interconnected by means of the cross. On the pins we set needle bearings which consist of a cover, safetyfuses, sleeve, needles and pickings which retain lubricant within the bearing. Those parts of the universal jointswhich are subjected to the most intense strains are between the other cross axles and the sleeves of the needlebearing. The asynchronous universal joint of the hinged type is illustrated in the Fig. 1, and consists of: 1-bearing needle, 2-ring, 3-cross joint, 4-fork complete with a flange, 5,6-grease-gun and valve and 7-forkcomplete with the shaft. Owing to unequal angle velocities of the driving and the driven shafts additional strainsof the above mentioned transmission parts (elements) occur, consequently, it is for this reason necessary to carryout experimental laboratory analyses and to determine the deformations of the above mentioned parts of the
Identification of changes in the microstructure of damaged elements spherical jointwww.ijeijournal.com Page | 39universal joint. Particularly interesting are the changes in the microstructure of the above mentioned parts whichoccur during the testings of the above mentioned universal joints in operation.III. LABORATORY ANALYSES OF THE MICROSTRUCTURE OF THE PARTS OFUNIVERSAL JOINTThe analyses of the microstructure were carried out on the optical microscope. The microstructuresappeared after the corrosion of the sample in the reagent 1% HNO3 in ethyl alcohol, and the observation wascarried out at the magnification X 625. The analysis was carried out on the necks of the cross axle and on thesleeves of the needle bearings. The picture of the microstructure of the cross-section of the neck is given in theFig. 2 and from the analysis of the photographic picture it is possible to see martensite + residual austenitewhich is not desirable in the cemented layer because of its lower hardness. This indicates that the thermaltreatment was not performed well. Most probably the sample was heated to a higher temperature during itstempering than it is allowable for this quality of treated steel which resulted in the increase of the austenite grainso that a certain quantity of austenite was retained between the martensite needles during the cooling.Figure 2: Neck sample; cross section; cemented layer,martensite + residual austeniteFigure 3: Neck sample; longitudinal section;cemented, layer; martensite + residual austeniteThe picture of the microstructure of the longitudinal section of the sleeve is given in the Fig. 3, andfrom the analysis of the photographic picture it can be seen that in the microstructure of the sleeve the cementiteis present on the grain border in the cemented layer in addition to martensite and the residual austenite. Thisphenomenon in the structure occurs at higher temperatures of cementing by means of carbonizing. Thesetemperatures are not appropriate for the quality of the given steel in which case higher carbon content on thesurface is achieved. This results in the separation of cementite on the borders of grains. In parallel to theappearance of cementite the grain increases too, which, in turn, increases the brittleness of the cemented layer.Figure 4: Sleeve sample; cemented layer on the outeredge; martensite + residual austenite + cementiteFigure 5: Sleeve sample; transit point between thecemented layer and the coreIV. THE POSSIBLE APPLICATION OF THE MACHINE VISION TECHNIQUESFor more quality identification of microstructure changes on parts of spherical joints, with the clasicallaboratory test we proposed the possible application of the machine vision to the microstructure analysis parts ofthe spherical joint. Improving basic inspection techniques may be accomplished by applying some new tools ordevices that make inspection points easier to see.
Identification of changes in the microstructure of damaged elements spherical jointwww.ijeijournal.com Page | 40Part of thespherical jointCCD imagesensorA/DconversionelectronicsEmbeddedprocessingelectronicsInterface MicroprocessorsystemDatabaseMonitor IntelligentsystemSUBJECTIlluminationDecreasing/increasing theillumination requirementsAnalogimage dataDigitalimage dataCompressedimage dataSoftware of MV formicrostructureanalysisPC PLATFORMCameracontrolOptic LenssystemFigure 6: Generic schema of MVS for MAMachine vision system will give us input information to intelligent system for microstructureanalysis.The structure of the proposed machine vision system for microstructure analysis (MVS for MA) isshown in Fig. 6. In the cadre of the microstructure changes we marked the presence of: austenite, martensite,benite, ferrite and etc. For that the size, shape and colour are key characteristics for visual monitoring change ofmicrostructure. It consists of next elements: microscope + CCD camera, PC platform – host processor system,software for microstructure condition monitoring- application software for end-user (developed GUI which userNeuro Inspector or IMAQ Vision functions as ActiveX control). Functional schema of proposed machine visionsystem is shown on Fig. 7. It consists from three functions: image capturing,, image processing and featuresextraction. Fig. 8 shows flowchart of MA (Microstructure Analysis) software development. The basic idea is todevelop a program which will be capable for automatic microstructure monitoring using image processingtechniques.ImagecapturingAOImageprocessingA1FeatureextractionA2PC PlatformMicroskope +cameraPart of thespherical jointSet of rules forimage capturingImageprocessingdefinitionReference features(features classes)Captured imageArithmetic operationsThresholdingColor Pattern MatchingBlob Analysis and MorphologyCountingIMAQ Vision Builder or NeuroInspector functionsProcessedimageInputs in anintelligentsystemLoadimage(i)STARTLoadreferentmasksINPUT DATAReferent image(s)Directory of saved images (i)IMAQ Visionfunctions orNeuro inspectorPixelvalue<Referentvaluei=i+1i<Number ofimagesENDTextmessageTextmessageDatabaseFigure 7: Functional schema of MV operations Figure 8: Flowchart of MA programV. USING COMPUTER VISION TECHNIQUES TO THE ANALYSES OF THEMICROSTRUCTUREThe analyses of the microstructure were carried out on the optical microscope. The microstructuresappeared after the corrosion of the sample in the reagent 1% HNO3 in ethyl alcohol, and the observation wascarried out at the magnification X 625. The analysis was carried out on the necks of the cross axle and on thesleeves of the needle bearings. The picture of the microstructure of the cross-section of the neck is given in theFig. 9 and from the analysis of the photographic picture it is possible to see martensite + residual austenitewhich is not desirable in the cemented layer because of its lower hardness. This indicates that the thermaltreatment was not performed well. Most probably the sample was heated to a higher temperature during itstempering than it is allowable for this quality of treated steel which resulted in the increase of the austenite grainso that a certain quantity of austenite was retained between the martensite needles during the cooling.
Identification of changes in the microstructure of damaged elements spherical jointwww.ijeijournal.com Page | 41Figure 9: Image preparationFor example it’s shown of the microstructure of the cross-section of the neck, which was for easiestanalysis converted into JPEG format (8 bits grayscale) in IMAQ Vision Builder 6.1 software . Other images,which are interesting for analyze of universal joint elements, are prepared and converted in the same imageformat Fig. 9. Image processing technique called BLOB (binary large objects) analysis is used for analyzing thestructure of joint elements.Figure 10: TresholdingFigure 11: Tresholding valuesNext steps have been performed: filtering the image to sharpen edges, separating particles from thebackground with tresholding Fig. 10, modifying blobs with morphological functions, analyzing the data.
Identification of changes in the microstructure of damaged elements spherical jointwww.ijeijournal.com Page | 42Figure 12: Advanced MorphologyFigure 13: Remove small objectsFigure 14: Particle analysisFigure 15: Measurement resultsMorphological operations prepare blobs in the image for quantitative analysis such as finding the area,perimeter, or orientation. Advanced Morphology technique is used for removing small objects that touch the
Identification of changes in the microstructure of damaged elements spherical jointwww.ijeijournal.com Page | 43border of the image Fig. 12. The measurement results are exported to Microsoft Excel for further analysis Fig.15.VI. CONCLUSIONSBase upon the performed laboratory analyses on the microstructure of the parts (elements) of theuniversal joints all the samples of their damages can be classified into the damages resulting from poormaintenance, wear during the operation and from poor construction and fabrication technology. Due to poorlyexecuted thermal - chemical treatments of the surfaces of the parts (elements) of the universal joints coarse-grained structures of lower hardness occur. This is illustrated by the picture of the microstructure of the crosssection of the parts (elements) of the universal joints and measured hardness values on individual parts of thesesections. This phenomenon is more pronounced on the elements in operation on which a sudden temperatureincrease occurs, and consequently, there are also the cases of noticeable plastic deformations in the form ofincreased width of impressions. Better quality cementation and greater depth of the cemented layer, as well as abetter quality tempering and the yielding (releasing) period can influence the condition of the material on thesurface and on the layer below the surface. In this way it is possible to achieve during the operation decreaseddamages on the parts (elements) of the universal joint as the integral part of the transmission mechanism. Besideof classical laboratory approach, this paper presents using of the computer vision techniques for the analysismicrostructure of the parts of universal joint. Quality of information got it on this way gave sharpen pictureabout microstructure changes of observed elements which are caused by action of complex loads.REFERENCES Sprečić D.; Mujanović E.: Analysis of the Wear a Conical Gear Pairs, and the Possibility of Applying Machine Vision to Analyzethe Microstructure, Intelligent technologies in logistics and mechatronics systems Itelms, Panevėžys, Lithuania, May 03-04, 2012,pp. 159-165. Williams J.A.: Engineering Tribology, Oxford University Press, 2005. Jain R.; Kasturi R.; Schunck G.B.: Machine Vision, McGraw-Hill, New York, 1995. Janičijević N.; Janković D.; Todorović I.: Konstrukcija motornih vozila, Beograd, Faculty of mechanical Engineering, 1998. Časnji F.; Klinar I.; Muzikravić V.: Savremene tendencije u automobilskoj tehnici – Mehaničke komponente i elektronskisistemi,Novi Sad, 2001. Klinar I.: Oprema motora SUS, Novi Sad, Faculty of technical science, 1995. Holmberg K.; Matthews A.: Coatings Tribology, Properties, Techniques and Applications in Surface Engineering, Amsterdam,1994.